Influence of Friction Stir Welding Parameters on Sliding Wear Behavior of
AA6061/0-10 wt.% ZrB2
in-situ Composite Butt Joints
I. Dinaharana*, N. Muruganb
Department of Mechanical Engineering, Karunya University, Coimbatore – 641114, Tamil Nadu, India.
Department of Mechanical Engineering, Coimbatore Institute of Technology, Coimbatore – 641014, Tamil Nadu, India.
Over the last decade attempts have been made to fabricate aluminum matrix composites (AMCs) reinforced with several ceramic particles. Aluminum reinforced with ZrB2 particles
is one such AMC. The successful application of new kind of AMCs lies in the development of secondary processes such as machining and joining. Friction stir welding (FSW) is a relatively new solid state welding which overcomes all the setbacks of fusion welding of AMCs. An attempt has been made to friction stir weld AA6061/ 0-10 wt. % ZrB2 in-situ
composites and to develop empirical relationships to predict the sliding wear behavior of butt joints. Four factors, five levels central composite rotatable design has been used to minimize the number of experiments. The factors considered are tool rotational speed, welding speed, axial force and weight percentage of ZrB2. The effect of these factors on wear rate (W) and
wear resistance (R) of the welded joints is analyzed and the predicted trends are discussed.
Key words: Metal matrix composite, Friction stir welding, Wear.
Adequate development of secondary processes such as cutting, forming, machining and joining of AMCs has not been fully established which limits its applications.
The presence of ceramic particles reduces the weldability of AMCs. Attempts to join AMCs using established fusion welding processes resulted in porosity, coarse microstructure, segregation and decomposition of ceramic particles and formation of brittle intermetallic compounds. The high temperature attained in fusion welding increases the tendency of ceramic particles to react with aluminum matrix. Achieving homogeneous distribution of ceramic particles in the weld zone was found to be difficult. The mechanical properties of the joints were poor [3-6]. Friction stir welding (FSW) is a promising candidate to join AMCs without fusion welding defects.
FSW was invented by The Welding Institute (TWI) in 1991. A non consumable rotating tool under sufficient axial force is plunged into the abetting edges of the plates to be joined and advanced along the line of the joint. The frictional heat generated by the tool softens the material and coalescence is achieved at the retreating side of the tool. The temperature rise during joining is well below the melting point . Though FSW is primarily developed to join aluminum alloys intense research has been extended to join other alloys such as magnesium, copper, brass, steel, nickel and titanium .
Availability of limited literatures reveals the lack of exploration on all aspects of FSW of AMCs. Earlier works were focused on FSW of aluminum reinforced with either Al2O3 or SiC [9-14]. Few works were reported on FSW of aluminum reinforced with B4C, TiB2, TiC and Mg2Si in the recent past [15-18]. Several researchers carried out FSW using a single set of parameters while few others attempted to study the influence of process parameters on joint properties. Prado et al.  examined the effect of rotational speed on tool wear of friction stir welded AA6061/20 vol % Al2O3 and observed that the tool wear was non linear. Shindo et al.  estimated the effect of welding speed on tool wear of friction stir welded A359/20 vol % SiC and noticed different degree of weld zone hardening. Vijay and Murugan  assessed the effect of different tool pin profiles on microstructural evaluation of friction stir welded AA6061/10 wt % TiB2 and found the square pin profile yielding higher tensile strength and finer grains in the weld zone. Nami et al.  analyzed the effect of tool rotational speed on microstructure and strength of friction stir welded Al/15 wt % Mg2Si and recorded different degree of weld zone hardening. Gopalakrishnan and Murugan  developed an empirical relationship to predict the strength of friction stir welded AA6061/ 3-7 wt % TiC and described the effect of welding speed, axial force, tool pin profile and weight percentage of TiC particles.
Lee et al.  compared the wear rate of friction stir welded AZ91/10 vol % SiC with parent composite and observed decrease in wear rate subsequent to FSW. However, he did not attempt to correlate the effect of FSW parameters on wear rate. This work is an attempt to develop empirical relationships to predict the sliding wear behavior of friction stir welded AA6061/0-10 wt % ZrB2 butt joints and analyze the influence of process parameters on wear rate and wear resistance of the welded joints. AA6061 has been used as matrix. Experiments were conducted according to central composite rotatable design. A number of researchers utilized central composite rotatable design to conduct experiments and developed precise empirical relationships to predict the influence of process parameters on the responses [18, 22-24].
2. SCHEME OF INVESTIGATION
2.1. Fabrication of AMCs
The AA6061-T6 rods (Ø25 mm) were melted in an electrical furnace using a graphite crucible. The chemical composition of AA6061 rods is presented in Table1. The weighed quantities of inorganic salts K2ZrF6 and KBF4 were added into the molten aluminum to produce ZrB2. The temperature of the melt was maintained at 8600C. The melt was stirred intermittently for 30 minutes. After removing slag the melt was poured into a preheated die. Castings were obtained with different weight percentage (0, 2.5, 5, 7.5 and 10 %) of ZrB2. A detailed fabrication procedure and formation of in-situ ZrB2 particles are available elsewhere .
Table 1: Chemical composition of AA6061-T6
Element Mg Si Fe Mn Cu Cr Zn Ni Ti Aluminum
wt.% 0.95 0.54 0.22 0.13 0.17 0.09 0.08 0.02 0.01 Balance
2.2. Identification of Process Variables
The predominant FSW process parameters which influence the joint properties are tool rotational speed (N), welding speed (S) and axial force (F) . The tool pin profile also plays a significant role on joint properties. A tool made of high carbon high chromium steel with square pin profile was used in this work . The dimensions of the tool are shown in Fig.1. The weight percentage of ceramic particles in the composite was reported to influence the joint properties [15, 18]. Hence, the weight percentage of ZrB2 particles (C) was also considered as a factor to understand its effects on sliding wear behavior.
2.3. Finding the Limits of the Process Variables
The FSW window for producing sound welds in AMCs is narrower compared to unreinforced alloys due to the presence of ceramic particles . A large number of trial welds were carried out to fix the working ranges of all selected process parameters. Each trial weld was inspected for smooth bead appearance and cross sectioned to verify the presence of defects such as pin hole, tunnel and worm hole in the weld zone. The limits of each process parameter were decided upon yielding defect free welds. The upper limit of a process parameter was coded as +2 and the lower limit was coded as –2 for the convenience of recording and processing experimental data. The coded values for intermediate values were calculated using the following relationship.
Xi = 2[2X – (Xmax + Xmin)] / (Xmax – Xmin) (1)
where Xi is the required coded value of a variable X; X is any value of the variable from Xmin to Xmax; Xmin is the lowest level of the variable; Xmax is the highest level of the variable. The decided levels of the selected process parameters with their units and notations are given in Table 2.
Table 2: Friction stir welding parameters and their levels
Levels No. Parameter Notation Unit
-2 -1 0 1 2
1 Rotational speed N rpm 1000 1075 1150 1225 1300
2 Welding speed S mm/min 30 40 50 60 70
3 Axial force F kN 4 5 6 7 8
4 Zirconium boride C wt.% 0 2.5 5 7.5 10
2.4. Developing the Design Matrix
Table 3: Design matrix and experimental results
FSW process parameters Trial
N S F C
Wear rate (x10-5 mm3/m)
T01 -1 -1 -1 -1 520 192 0.88
T02 +1 -1 -1 -1 501 200 0.84
T03 -1 +1 -1 -1 507 197 0.85
T04 +1 +1 -1 -1 532 188 0.90
T05 -1 -1 +1 -1 500 200 0.84
T06 +1 -1 +1 -1 524 191 0.88
T07 -1 +1 +1 -1 514 195 0.87
T08 +1 +1 +1 -1 527 190 0.89
T09 -1 -1 -1 +1 373 268 0.91
T10 +1 -1 -1 +1 368 272 0.90
T11 -1 +1 -1 +1 374 267 0.92
T12 +1 +1 -1 +1 382 262 0.94
T13 -1 -1 +1 +1 357 280 0.88
T14 +1 -1 +1 +1 379 264 0.93
T15 -1 +1 +1 +1 352 284 0.86
T16 +1 +1 +1 +1 381 262 0.93
T17 -2 0 0 0 460 217 0.90
T18 +2 0 0 0 492 203 0.96
T19 0 -2 0 0 481 208 0.94
T20 0 +2 0 0 457 219 0.90
T21 0 0 -2 0 459 218 0.90
T22 0 0 +2 0 474 211 0.93
T23 0 0 0 -2 524 191 0.80
T24 0 0 0 +2 265 377 0.77
T25 0 0 0 0 423 236 0.83
T26 0 0 0 0 438 228 0.86
T27 0 0 0 0 418 239 0.82
T28 0 0 0 0 441 227 0.86
T29 0 0 0 0 435 230 0.85
T30 0 0 0 0 411 243 0.81
T31 0 0 0 0 421 238 0.83
Plates of size 100 mm X 50 mm X 6 mm were prepared from the castings. The butt welding of AA6061- ZrB2 composites was carried out automatically in an indigenously built FSW machine (M/s RV Machine Tools, Coimbatore, INDIA). The welding was carried out as per design matrix at random to eliminate any systematic errors creeping into the system. The tool was plunged into the abutting surfaces until the shoulder touched the surface of the plates. The machine table was advanced at the set welding speed after a short dwell period. The dwell period serves the purpose of generating the required heat to initiate plastic flow of the material. Typical welded plates of trial run 23 and 24 are shown in Fig.2.
Figure 2: Photograph showing typical friction stir welded plates: a) T23 and b) T24.
2.6. Recording the Response Parameters
Specimens of size 6 mm x 6 mm x 50 mm were extracted from each welded plate. The dry sliding wear behavior was measured using a pin-on-disc wear apparatus (DUCOM TR20-LE) at room temperature according to ASTM G99-04 standard. The polished surface of the pin was slid on a hardened chromium steel disc. The test was carried out at a sliding velocity of 1.5 m/s, normal force of 25 N and sliding distance of 2500 m. The wear parameters were selected to yield an appreciable steady state wear based on trial experiments. A computer-aided data acquisition system was used to monitor the loss of height. The volumetric loss was computed by multiplying the cross section of the test pin with its loss of height. The wear rate (W) and wear resistance (R) were calculated  as follows and given in Table 3.
W (mm3/m) = Volumetric loss / Sliding distance (2)
R (m/mm3) = 1 / Wear rate (3)
The sliding wear behavior of the parent composite was also measured at the same wear parameters and presented in Table 4. The relative wear rate was computed as given below and presented in Table 3.
Table 4: Sliding wear behavior of AA6061/ZrB2 in-situ composites
Wear rate (x10-5 mm3/m)
Wear resistance (m/mm3)
0 657 152
2.5 594 168
5 510 196
7.5 408 245
10 345 290
2.7. Development of Empirical Relationships
The response functions representing the wear rate and wear resistance of friction stir welded plates are functions of tool rotational speed (N), welding speed (S), axial force (F) and weight percentage of ZrB2 (C) can be expressed as
W = f (N, S, F, C) (5)
R = f (N, S, F, C) (6)
The second order polynomial regression equation used to represent the response surface ‘Y’ for K factors is given by k k k Y= b0 + ∑ bixi +∑ biixi2 +∑ bijxixj (7)
i=1 i=1 i=1 where b0 is the average of responses and bi, bii and bij are the coefficients which depend on respective main and interaction effects of the parameters. The values of the coefficients were estimated using the following expressions . b0 = 0.142857(∑Y) – 0.035714∑∑ (XiiY) (8)
bi = 0.041667 ∑ (XiY) (9)
bii = 0.03125∑ (XiiY) + 0.00372 ∑∑ (XiiY) – 0.035714(∑Y) (10)
bij = 0.0625∑ (XiiY) (11)
The selected polynomial for four factors could be expressed as W = b0 + b1 (N) + b2 (S) + b3 (F) + b4 (C) + b11 (N2) + b22 (S2) + b33 (F2) + b44 (C2) + b12 (NS) + b13 (NF) + b14 (NC) + b23 (SF) + b24 (SC) + b34 (FC) (12)
R = b0 + b1 (N) + b2 (S) + b3 (F) + b4 (C) + b11 (N2) + b22 (S2) + b33 (F2) + b44 (C2) + b12 (NS) + b13 (NF) + b14 (NC) + b23 (SF) + b24 (SC) + b34 (FC) (13)
affecting the accuracy of the empirical relationships using t-test. The significant coefficients were taken into account to construct the final empirical relationships. The developed final empirical relationships with FSW parameters in coded form are given below.
W = 426.714 + 6.708N – 0.042S + 0.292F – 69.875C + 10.936N2 + 9.186S2 + 8.561F2
R = 234.429 – 3.417 N + 0.25F + 40.75C – 5.857N2 – 4.982S2 – 4.732F2
+ 12.643C2 (15)
2.8. Checking the Adequacy of the Empirical Relationships
The statistical results of the developed empirical relationships are presented in Table 5. The predicted empirical relationship values will exactly match with the experimental results if R-Square value is 1. The higher values of ‘R-R-Square’ and lower values of standard error (SE) indicate that the empirical relationships are quite adequate and can be used to predict the responses (W and R) without appreciable error. The adequacy of the developed empirical relationships was also tested using the analysis of variance (ANOVA) technique which is presented in Table 6. The calculated values of F-ratio are greater than the tabulated values at 95% confidence level which means the developed empirical relationships are considered to be adequate. Further the validity of the empirical relationships is tested by drawing scatter diagrams as shown in Fig. 3. The experimental values and predicted values from the empirical relationships are scattered both sides and close to 450 line which indicate the perfect fitness of the developed empirical relationships.
Table 5: Statistical results
Response R-square Adjusted R-square
W 0.976 0.967 12.002
R 0.976 0.968 7.26
Table 6: ANOVA results
Response Source Sum of squares Degrees of freedom Mean-square F-ratio (calculated) F-ratio (tabulated)
W Regression 129030.468 8 16128.81 111.97 2.40
Residual 3168.887 22 144.04
R Regression 47836.646 8 5979.581 113.45 2.40
Residual 1159.548 22 52.707
2.9. Validation of the Empirical Relationships
calculated as [(experimental value – empirical relationship value) / empirical relationship value] X 100. It is found from the table that the error is within ± 7% which confirms the accuracy of the developed empirical relationships.
Figure 3: Scatter diagram for the developed empirical relationships: (a) Wear rate and (b) Wear resistance.
Table 7: Results of conformity experiments
Wear rate (x10-5 mm3/m) Wear resistance (m/mm3) FSW process
N S F C
1 1.25 -1.50 -1.25 -2 610.43 587.92 3.83 163.82 171.16 -4.29
2 0.75 -0.25 0.5 -1 525.78 501.20 4.90 190.19 199.10 -4.47
3 0.25 -0.75 1.5 0 425.05 453.97 -6.37 235.27 220.13 6.88
4 -0.5 0.75 0.75 1 378.56 356.95 6.05 264.16 282.79 -6.59
5 -1.5 -1.25 -0.5 2 270.35 280.15 -3.50 369.89 349.36 5.88
2.10. Wear Surface Morphology
Wear surface of selected specimens were observed using scanning electron microscope (JEOL-JSM-6390).
3. RESULTS AND DISCUSSIONS
mechanically. Each parameter independently contributes to frictional heat generation in addition to stirring, extruding and forging the plasticized material.
The effects of process parameters such as tool rotational speed, welding speed, axial force and weight percentage of ZrB2 on sliding wear behavior of friction stir welded AA6061-ZrB2 in-situ composites are evaluated using the developed empirical relationships. The trends obtained for each process parameter are represented in Figs.4-7. The possible causes for the effects of different process parameters on sliding wear behavior are elaborated as follows.
3.1. Effect of Tool Rotational Speed
Fig.4 shows the sliding wear behavior of friction stir welded AA6061-ZrB2 in-situ composites as a function of tool rotational speed. The wear rate decreases as tool rotational speed increases and reaches minimum at 1125 rpm. Further increase in tool rotational speed leads to increased wear rate. The wear resistance follows an inverse trend of wear rate as estimated.
Figure 4: Effect of tool rotational speed on sliding wear behavior.
The tool rotation generates frictional heat as well as stirring and mixing of material around the tool pin. Optimum stirring and sufficient heat generation is required to produce sound joints with fine recrystallized grains. When this condition is achieved during welding the joints produced will exhibit highest wear resistance. Increase in frictional heat generation is observed with increase in tool rotational speed. Lower heat input condition prevails at lower tool rotational speeds (1000 rpm and 1075 rpm) which are also associated with lack of stirring. The net result is poor consolidation of material which leads to poor wear resistance at lower tool rotational speeds.
3.2. Effect of Welding Speed
Fig.5 shows the sliding wear behavior of friction stir welded AA6061-ZrB2 in-situ composites as a function of welding speed. The wear rate decreases as welding speed increases and reaches minimum at 50 mm/min. Further increase in welding speed leads to increased wear rate. The wear resistance follows an inverse trend of wear rate as estimated.
The rotating tool stirs the material as discussed earlier. The welding speed prompts the translation of tool which in turn pushes the stirred material from front to the back of the tool pin and completes the welding. The rubbing of tool shoulder and pin with the work piece generates frictional heat. The welding speed determines the exposure time of this frictional heat per unit length of weld and subsequently affects the grain growth . Optimum exposure time and translation of stirred material will lead to good consolidation of material with fine grains. Joints experience such condition during welding will exhibit higher wear resistance.
Figure 5: Effect of welding speed on sliding wear behavior.
3.3. Effect of Axial Force
Fig.6 shows the sliding wear behavior of friction stir welded AA6061-ZrB2 in-situ composites as a function of axial force. The wear rate decreases as axial force increases and reaches minimum at 6 kN. Further increase in axial force leads to increased wear rate. The wear resistance follows an inverse trend of wear rate as estimated.
Figure 6: Effect of axial force on sliding wear behavior.
Frictional heat generated between the tool shoulder and the surface of the plate to be welded is dependent upon the coefficient of friction which is decided by the axial force. Optimum frictional heat coupled with sufficient extrusion of plasticized material is required to produce sound joints. When this condition is encountered during welding the joint will yield higher wear resistance. When axial force increases frictional heat generation also increases. Lower heat is generated at lower axial forces (4 kN and 5 kN) as well as cause improper consolidation of material. Micro voids appear at lower axial forces which leads to poor wear resistance at lower axial forces. Higher heat is generated exceeding the desired level at higher axial forces (7 kN and 8 kN). The plunge depth of the tool into the welded plate is higher at higher axial forces. Further the flash level increases with increased axial force. Increased flash level causes local thinning of welded plate leading to poor wear resistance at higher axial forces.
3.4. Effect of ZrB2 Particles
Fig.7 shows the sliding wear behavior of friction stir welded AA6061-ZrB2 in-situ composites as a function of weight percentage of ZrB2 particles. The wear rate decreases with increase in ZrB2 content while the wear resistance follows an inverse trend as estimated. The joints fabricated at N = 1150 rpm, S = 50 mm/min and F = 6 kN show higher wear resistance. Good consolidation of material with optimum stirring and adequate heat generation may be taking place at this combination of parameters.
Figure 7: Effect of weight percentage of ZrB2 on sliding wear behavior.
The inherent characteristic of applying FSW to ceramic particulate reinforced metal matrix composites is the ability to provide identical distribution of ceramic particles in the weld zone to that of parent composite. The weight percentage of ZrB2 particles was considered as a process parameter to substantiate this statement. Figs.8-9 reveal the microstructure of parent composite and weld zone of joints which have different weight percentage of ZrB2 particles. The specimens were prepared as per standard metallographic procedure and color etched with 1 g NaOH, 4 g KMnO4 in 100 ml distilled water. ZrB2 particles appear as white and circular in shape. The reaction of K2ZrF6 with KBF4 produced ZrB2 particles at varying sizes. The uniform distribution of ZrB2 particles in the welded joints irrespective of weight percentage is explicit.
3.5. Effect of FSW
Figure 8: Photomicrographs of base composites containing ZrB2: a) 0% (T23); b) 2.5% (T01); c) 5% (T29); d) 7.5% (T15) and e) 10% (T24).
3.6. Wear Surface Morphology
wear surface temperature which causes plastic deformation and dislocation in the inner surface of the composites.
Figure 9: Photomicrographs of Weld zone of AMCs containing ZrB2: a) 0% (T23); b) 2.5% (T01); c) 5% (T29); d) 7.5% (T15) and e) 10% (T24).
the frictional heat softens the surface layer. The difference in thermal expansion coefficient between the matrix and the ZrB2 particles creates the interface stress. When the interface stress exceeds the bond strength the particles are pulled off. The pulled off particles begin to act as wear particles in the sliding wear course.
Figure 10: SEM micrograph of wear surface of specimens with: a) 0 wt.% ZrB2 (T23); b) 2.5 wt.% ZrB2 (T02); c) 5.0 wt.% ZrB2 (T30); d) 7.5 wt.% ZrB2 (T11) and e) 10 wt.% ZrB2
The following conclusions are derived from the present work:
• Empirical relationships incorporating the welding parameters are developed to predict the sliding wear behavior of AA6061/0-10 wt.% ZrB2 in-situ composite butt welded joints.
• The process parameters independently influence the sliding wear behavior over the entire range of parameters studied.
• The joints fabricated at N = 1150 rpm, S = 50 mm/min and F = 6 kN yields highest wear resistance.
• A homogeneous distribution of ZrB2 particles in the welded joints irrespective of weight percentage is observed.
• FSW enhances the wear resistance of the developed AMCs
• A change in the wear mode from adhesion wear to abrasive wear with the increase in weight percentage of ZrB2 particles is observed.
The authors are grateful to the Management and Department of Mechanical Engineering, Coimbatore Institute of Technology, Coimbatore, India for extending the facilities to carry out this investigation. The authors acknowledge the financial support rendered by All India Council for Technical Education, Govt. of India. The corresponding author acknowledges the INSPIRE fellowship awarded by Department of Science and Technology, Govt. of India. Authors are also thankful to Mr.S.J.Vijay, Mr.K.Kalaiselvan, Mr.B.Ashok Kumar, Mr.A.Raja, Mr. A. Samson Ratnakumar, Mr. S.Vijaya Ganesh, Mr. Palanisamy and Mr. Mahalingam for their assistance.
 Miracle, D.B. , 2005, “Metal matrix composites – From science to technological significance”, Composites Science and Technology, Vol.65, pp. 2526–2540.  Rosso, M., 2006, “Ceramic and metal matrix composites: Routes and properties”,
Journal of Materials Processing Technology, Vol.175, pp. 364–375.
 Huang, R.Y. , Chen, S.C. , Huang, J.C., 2001,“Electron and Laser Beam Welding of High Strain Rate Superplastic Al-6061/SiC Composites”, Metallurgical and Materials Transactions A, Vol.32, pp.2575-2584.
 Storjohann, D. , Barabash, O.M. , Babu, S.S., David, S.A., Sklad, P.S., Bloom, E.E., 2005, “Fusion and Friction Stir Welding of Aluminum-Metal-Matrix Composites”, Metallurgical and Materials Transactions A, Vol.36, pp.3237-3247.
 Bassani, P., Capello, E., Colombo, D., Previtali, B., Vedani, M., 2007, “Effect of process parameters on bead properties of A359/SiC MMCs welded by laser”, Composites: Part A, Vol.38, pp.1089–1098.
 Mishra, R.S., Ma, Z.Y., 2005, “Friction stir welding and processing”, Materials Science and Engineering R, Vol.50, pp.1–78.
 Nandan, R., Roy, T.D., Bhadeshia, H. K. D. H., 2008, “Recent Advances in Friction Stir Welding – Process, Weldment Structure and Properties”, Progress in Materials Science, Vol.53, pp.980-1023.
 Prado, R.A. , Murr, L. E. , Shindo, D. J., Soto, K.F., 2001, “Tool wear in the friction-stir welding of aluminum alloy 6061+20% Al2O3: a preliminary study”, Scripta materialia, Vol.45, pp.75-80.
 Shindo, D. J., Rivera, A. R., Murr, L. E., 2002, “Shape optimization for tool wear in the friction-stir welding of cast AI359-20% SiC MMC”, Journal of Materials Science, Vol.37, pp. 4999 – 5005.
 Marzoli L.M., Strombeck, A.V., Santos, J.F. D, Gambaro, C. , Volpone, L.M., 2006, “Friction stir welding of an AA6061/Al2O3/20p reinforced alloy”, Composites Science and Technology,Vol.66, pp.363–371.
 Amirizad, M., Kokabi, A.H., Gharacheh, M. A, Sarrafi, R., Shalchi, B., Azizieh, M., 2006, “Evaluation of microstructure and mechanical properties in friction stir welded A356+15%SiCp cast composite”, Materials Letters, Vol.60, pp.565–568.
 Ceschini, L., Boromei, I., Minak, G., Morri, A., Tarterini, F., 2007, “Effect of friction stir welding on microstructure, tensile and fatigue properties of the AA7005/10
vol.%Al2O3p composite”, Composites Science and Technology, Vol.67, pp.605–615.  Feng, A.H., Xiao, B.L., Ma, Z.Y., 2008, “Effect of microstructural evolution on
mechanical properties of friction stir welded AA2009/SiCp composite”, Composites Science and Technology, Vol.68, pp.2141–2148.
 Chen, X.G., Silva, M. D., Gougeon, P., Georges, L. S., 2009, “Microstructure and mechanical properties of friction stir welded AA6063–B4C metal matrix composites”, Materials Science and Engineering A, Vol.518, pp.174–184.
 Vijay, S.J., Murugan, N., 2010, “Influence of tool pin profile on the metallurgical and mechanical properties of friction stir welded Al–10 wt.% TiB2 metal matrix composite”, Materials and Design, Vol.31, pp.3585–3589.
 Nami, H., Adgi, H., Sharifitabar, M., Shamabadi, H., 2010 “Microstructure and mechanical properties of friction stir welded Al/Mg2Si metal matrix cast composite”, Materials and Design,Vol.32, pp.976–983.
 Gopalakrishnan, S., Murugan, N., 2011, “Prediction of tensile strength of friction stir welded aluminum matrix TiCp particulate reinforced composite”, Materials and Design, Vol.32, pp.462–467.
HfB2 and TiSi2”, International Journal of Refractory Metals and Hard Materials, Vol.29, pp.21–30.
 Guo, S.Q., Kagawa, Y., Nishimura, T., 2009, “Mechanical behavior of two-step hot-pressed ZrB2-based composites with ZrSi2”, Journal of the European Ceramic Society, Vol.29, pp.787–794.
 Lee, W.B., Lee, C.Y., Kim, M.K., Yoon, J., Kim, Y.J, Yoen, Y.M., Jung, S.B., 2006, “Microstructures and wear property of friction stir welded AZ91 Mg/SiC particle reinforced composite”, Composites Science and Technology, Vol.66, pp.1513–1520.  Elangovan, K., Balasubramanian, V., Babu, S., 2009, “Predicting tensile strength of
friction stir welded AA6061 aluminum alloy joints by a mathematical model”, Materials and Design, Vol.30, pp.188–193.
 Sundaram, N. S., Murugan, N., 2010, “Tensile behavior of dissimilar friction stir welded joints of aluminum alloys”, Materials and Design, Vol.31, pp.4184–4193.
 Kumar, S., Balasubramanian, V., 2010, “Effect of reinforcement size and volume fraction on the abrasive wear behaviour of AA7075Al/SiCp P/M composites—A statisticalanalysis”, Tribology International, Vol.43, pp. 414–422.
 Kumar, G.N., Narayanasamy, R., Natarajan, S., Babu, S.P. K., Sivaprasad, K.,
Sivasankaran, S., 2010, “Dry sliding wear behavior of AA 6351-ZrB2 in situ composite at room temperature”, Materials and Design, Vol.31, pp.1526–1532.
 Mandal, A., Chakraborty, M., Murty, B.S., 2007, “Effect of TiB2 particles on sliding wear behaviour of Al–4Cu alloy”, Wear, Vol.262, pp.160–166.
 Box, G.E.P., Hunter, W.H, Hunter, J.S., 1978, “Statistics for experiments”, Ed.10, Wiley, NewYork.
 Karthikeyan, L., Senthilkumar, V.S., Padmanabhan, K.A., 2010, “On the role of process variables in the friction stir processing of cast aluminum A319 alloy”, Materials and Design,Vol.31, pp.761–771.
 Cavaliere, P., Squillace, A., Panella, F., 2008, “Effect of welding parameters on mechanical and microstructural properties of AA6082 joints produced by friction stir welding”, Journal of Materials Processing Technology, Vol.200, pp.364–372.  Kumar, K., Kailas, S.V., 2008, “On the role of axial load and the effect of interface